more appropriate to describe the low cyclic stress-strain curve than the known Hollomon equation. On basis of theﬁtting equation, the low cyclic stress-strain curve could be validly predicted via merely knowing the material’s engineering stress-strain curve and the stabilized cyclic stresses at two strain amplitudes. The feasibilities of theﬁtting method and prediction method were veriﬁed by the low cycle fatigue tests on extruded AZ31B magnesium alloy, 7075 aluminum alloy and H63 copper zinc alloy. The predicted and actual stabilized cyclic stresses were approximately close to each other. From engineering standpoint, the prediction method would reduce the testing work amount of cyclic stress-strain curve to a great extent. [doi:10.2320/matertrans.M2015085]

(Received March 2, 2015; Accepted April 10, 2015; Published June 25, 2015)

Keywords: cyclic stress-strain curve, tensile, fatigue, AZ31B magnesium alloy

1. Introduction

Depending on the ratio of monotonic ultimate tensile
strength to the yield strength, a metal may undergo cyclic
hardening, cyclic softening or remain cyclically stable. Cyclic
hardening would lead to a decreasing peak strain with
increasing cycles and cyclic softening would lead to a
continually increasing strain range and early fracture.1)_{For}

the materials with cyclic hardening behavior, the hysteresis
loops always stabilize within about 100 cycles then the
materials reach to a stabilized condition. The cyclic
stress-strain curve is usually determined by connecting the tips of
stable hysteresis loops from the low cyclic fatigue testing
at various strain amplitudes.1,2) _{Therefore, the cyclically}

stabilized stress-strain curves do not coincide with static engineering stress-strain curves with different degrees of stress differences.3,4) Generally, to accurately describe the cyclic stress-strain curves, abundant stable hysteresis loops at various strain amplitudes are expected, and that would lead to a great many work amount. If the low cyclic stress-strain curve could be predicted combining with the engineering stress-strain curve and merely several stable hysteresis loops, the work amount would be simpliﬁed to a great extent.5)

Additionally, there are two common mathematical
descrip-tions of the work hardening phenomenon.1) _{Speci}_{ﬁ}_{cally,}

Hollomon equation is a power law relationship and is frequently used to describe the true tensile stress-strain curve of materials at the region of uniform plastic deformation:

·¼Kð¾pÞn ð1Þ

Wherenis the strain-hardening exponent,Kis the strength coefﬁcient, ¾pis the plastic strain, and ·is the stress. Ratke

et al.6)had reported that Hollomon equation was reliable in large strain area rather than in small strain area. Another common variation which includes the yield stress is the Ludwik equation as shown in eq. (2):

· ¼·oþKð¾pÞn ð2Þ

Where·ois the yield stress, andK,n,¾pand·are the same

parameters as shown in eq. (1). The strength coefﬁcientKis structure dependent and is inﬂuenced by the processing of materials, and for most metals,nhas values between 0.1 and 0.5. The strain-hardening exponentn could by described as:

n¼dðln·Þ

dðln¾Þ ¼ ¾ ·

d·

d¾ ð3Þ

Although the typical cyclic stress-strain curve could be
described by an analogy with Hollomon equation or Ludwik
equation based on exponential ﬁtting, the ﬁtting precision
might not be high enough with unsatisfactory correlation
coefﬁcient if the stable hysteresis loops is insufﬁcient. As
basic methods of static and dynamic mechanical tests,
the tensile and low cycle fatigue tests have been widely
adopted to determine the basic mechanical properties of
structural materials.712) Take the extruded AZ31B
magne-sium alloy812) with typical cyclic hardening behavior for
example, S. Hasegawa et al.10) investigated the low cycle
fatigue behavior under uniaxial cyclic loading by both strain
and stress controlled conditions, and a fatigue life evaluation
method was discussed based on Manson-Cofﬁn equation, and
Y. C. Lin et al.11) _{studied the hot tensile deformation and}

fracture behaviors, and the effects of deformation parameters on the strain hardening rate, strain rate sensitivity, micro-structural evolution and fracture morphology were also discussed. However, the quantitative relationships between the static and cyclic stress-strain curves of AZ31B magne-sium alloy were seldom mentioned.

This paper focused on the prediction method of cyclic stress-strain curves via merely knowing the material’s stabilized cyclic stresses at two strain amplitudes and the engineering stress-strain curve, and a ﬁtting method was developed based on exponentialﬁtting to describe the static and cyclic stress-strain curves.

2. Exponential Fitting Method

For structural materials with cyclic hardening behaviors, both the engineering and cyclic stress-strain curves monoton-ically increased at region of uniform plastic deformation, on

condition that the two curves could be ﬁtted by similar functions, the cyclic curve could be deduced by the engineering curve theoretically. Meanwhile, although the stress-strain curve of many metals in the region of uniform plastic deformation could be described by the classical Hollomon equation, the equation might not be absolutely appropriate to describe the engineering stress-strain curve. The engineering stress-strain curve does not give a true indication of the deformation characteristics, because it is based entirely on the original dimensions of the specimen, and these dimensions would change continuously during the tensile test. Actually, the true stress-strain curve13) presents a larger stress value compared with the engineering curve as the cross-sectional area of the specimen is gradually decreasing.

To describe the engineering curve at the materials’typical plastic deformation stage, a miniaturized self-made device with separate modular tensile and fatigue actuators was developed. The loading principle, function, gripping method and advantages of the device have been reported in detail in the previous work.14)The prototype of the proposed device with speciﬁc dimensions of 158 mm©124 mm©43 mm is shown in Fig. 1. The tensile actuator was mainly consisted of a servo motor (Maxon EC-max) with a large reduction ratio gear reducer, a two-stage worm gears reducer, a load sensor (SM 609-A) with measurement range of 1000 N and a displacement sensor (SDVH8B) with measurement range of 10 mm and resolution of 1 µm. The fatigue actuator was mainly consisted of a specialﬂexure hinge and a piezoelectric stack. The compatibility with tensile actuator was realized by a couple of positioning pins, which were assembled on the rigid part of theﬂexure hinge. Therefore, the fatigue actuator could not only work independently but also combine with the tensile actuator to output tensile/fatigue combined loads.

Figure 2 shows the engineering stress-strain curve of an extruded AZ31B magnesium alloy, and the alloy composition of the magnesium alloy was determined by energy dispersive spectrometer (Inca X-Max, Oxford Instruments, United Kingdom) and shown in Table 1. Based on the obtained engineering stress-strain curve, a novel equation based on a modiﬁed exponentialﬁtting method was proposed and shown in eq. (4), whereAis the strength coefﬁcient,bis the strain-hardening exponent, c is the constant term, ¾p is also the

plastic strain, and ·f is theﬁtted stress value.

For the plastic strain range from the yield strain to 0.02 (part i as shown in Fig. 2), which could be considered as the

range of cyclic strain amplitude for many structural materials that are subjected to low cycle fatigue loads, the local engineering stress-strain curve was ﬁtted and shown as eqs. (5) and (6) by respectively using the Hollomon equation and the modiﬁed ﬁtting equation. As shown in Fig. 2, on basis of eq. (5), the ﬁtting result was inconsistent with the actual engineering curve, while, when the curve was ﬁtted by the modiﬁed equation, the ﬁtted and actual engineering curves were approximate with correlation coefﬁcient of 0.9998. Therefore, the modiﬁed equation could be considered as more appropriate to describe the engineering curve at region of uniform plastic deformation than the Hollomon equation.

·f ¼Ae ¾p

b þC ð4Þ

· ¼557:2ð¾pÞ0:2412 ð5Þ ·f ¼ 160:2e

¾p

0:0052þ210:4 ð6Þ

On the other hand, although the typical cyclic stress-strain curves could also be described by the Hollomon equation, the

ﬁtting precision might not be high enough with unsatisfactory correlation coefﬁcient, especially for the insufﬁcient stabi-lized hysteresis loops. Seen from eq. (4), theoretically, the

ﬁtted cyclic stress-strain curve could be obtained based on merely three stabilized hysteresis loops, in other words, if the stabilized cyclic stresses could be accurately calculated by merely three strain amplitudes and stabilized stresses, the work amount to obtain the cyclic stress-strain curve would be signiﬁcantly reduced. To investigate the feasibility of the proposed ﬁtting method, the stabilized cyclic stresses at various strain amplitudes were tested by using the proposed tensile-fatigue device. During the tests, the low cycle fatigue loading rate, namely the tensile and compressive rate, was set as constant 5 µm/s. When the strain amplitude was 0.0058, the stabilized cyclic stress under stable condition was 182.1 MPa, when the strain amplitude increased to 0.014, the

Fig. 1 Prototype of the proposed device including with a compact piezoelectric actuator.

Fig. 2 Fitting results by respectively using the Hollomon equation and the modiﬁed ﬁtting equation to be compared with the actual engineering stress-strain curve of an extruded AZ31B magnesium alloy.

Table 1 Alloy composition of AZ31B magnesium alloy.

Element Mg Cu Zn Mn Al Fe

stabilized cyclic stress of 227.2 MPa was obtained. Compar-ing with the engineerCompar-ing stress-strain curve as shown in Fig. 2, with the identical strain amplitudes, the stabilized cyclic stresses were higher than the tensile stresses, which indicated the extruded AZ31B magnesium alloy presented obvious cyclic hardening behavior. Similarly, by respectively adopting the Hollomon equation and the modiﬁed equation, theﬁtting results of low cyclic stress-strain curves are shown in Fig. 3. The coupled strain amplitudes and stabilized cyclic stresses were 0.0058, 182.5 MPa, 0.011, 216.8 MPa, and 0.014, 227.2 MPa. Based on the Hollomon equation, when adopting 0.0058 and 0.011 as strain amplitudes, the ﬁtting result is shown in eq. (7), and eq. (8) also shows the ﬁtting result when adopting 0.011 and 0.014 as strain amplitudes, the two ﬁtted curves incompletely coincided with the stabilized cyclic stresses and could not accurately reﬂect the actual cyclic stress-strain curve. For the identical known parameters, theﬁtting result by using the modiﬁed exponen-tial ﬁtting method is shown in eq. (9), and the correlation coefﬁcient was obtained as 0.9997. Therefore, the proposed

ﬁtting equation was also available to describe the cyclic stress-strain curve at region of uniform plastic deformation.

·¼707:2ð¾pÞ0:2621 ð7Þ ·¼430:5ð¾pÞ0:1517 ð8Þ ·f ¼ 155:2e

¾p

0:0056þ238:6 ð9Þ

3. Results and Discussions

Although the cyclic stress-strain curve could be deduced by merely three stabilized cyclic stresses at respective strain amplitude on basis of the proposed ﬁtting method, accurate prediction method with less known stabilized cyclic stresses provided was expected. Now that the proposedﬁtting method was appropriate for the description of both the engineering and cyclic stress-strain curves, and the engineering and cyclic stress-strain curves presented the same exponential trend of monotonic increasing at region of uniform plastic deforma-tion, therefore, the mathematic relation between the engineer-ing and cyclic stress-strain curves could be established. The mathematic expression should include a constant term and an

exponential term related to the independent variable (plastic strain¾p), the exponential term and constant term were used

to adjust the shape and amplitude of the curve respectively. Equation (10) shows the proposed prediction method of cyclic stress-strain curve, where·cis the predicted stabilized

cyclic stress, ·c1 and ·c2 are the known stabilized cyclic

stresses at two strain amplitudes, ·m1 and ·m2 are the

corresponding static stresses,kcis the exponential adjustment

coefﬁcient,tcis the cyclic constant term,¾pis also the plastic

strain and ·m is the static stress. On condition that·c1, ·c2,

·m1,·m2and¾pwere all known parameters,kcandtccould be

calculated accordingly. Theoretically, the prediction method merely required the material’s two stabilized cyclic stresses at respective strain amplitudes and the engineering stress-strain curve, which are not difﬁcult to obtain from the low cycle fatigue and uniaxial tensile tests respectively. By using eq. (10), the prediction result of low cyclic stress-strain curve of the extruded AZ31B magnesium alloy compared with the stabilized cyclic stresses at given strain amplitudes is shown in Fig. 4. The given strain amplitudes were 0.0058 and 0.014, the corresponding stabilized cyclic and static stresses were 182.5 MPa, 227.2 MPa and 161.5 MPa, 202.5 MPa respec-tively, sokcandtccould be respectively calculated as 0.0971

and ¹10.2. Meanwhile, based on eq. (10), when the strain amplitudes was 0.011, the predicted stabilized cyclic stress was 218.1 MPa, as above mentioned, the actual stabilized cyclic stress obtained from the low cyclic fatigue test was 216.8 MPa, so the predicted and actual stresses were approximately close. Additionally, the actual cyclic stress-strain curve of the magnesium alloy on basis of more plentiful strain amplitudes at region of uniform plastic deformation was experimentally obtained. As shown in Fig. 5, the predicted curve was also from the engineering stress-strain curve and the known cyclic stresses above mentioned. For the strain range from 0.0058 to 0.02, the predicted and actual low cyclic stress-strain curves were approximate with correlation coefﬁcient of 0.9988. There-fore, the feasibility of the prediction method was prelimi-narily veriﬁed.

·c¼1_{2} _{·}·c1

m1þ ·c2 ·m2

ekc¾p·mþt_{c} ð10Þ

Fig. 3 Fitting results of cyclic stress-strain curve by using variousﬁtting methods.

Furthermore, to verify the universal feasibility of the prediction method, 7075 aluminum alloy and H63 copper zinc alloy were adopted to obtain the predicted stabilized cyclic stresses. Speciﬁcally, for 7075 aluminum alloy as shown in Fig. 6(a), the strain range was from 0.0052 to 0.043. For the three given strain amplitudes, 0.008, 0.024 and 0.039, the predicted stabilized cyclic stresses ·c were

543.6 MPa, 573.6 MPa and 596.3 MPa respectively, mean-while, the corresponding stabilized cyclic stresses·sdirectly

obtained from the low cyclic fatigue tests were 542.1 MPa,

574.5 MPa and 597.5 MPa respectively, the maximum predicted stress error for the three strain amplitudes was only 1.5 MPa. On the other hand, for H63 copper zinc alloy as shown in Fig. 6(b), the strain range was from 0.0053 to 0.031. On basis of strain amplitudes of 0.007, 0.019 and 0.030, the corresponding ·c were 324.1 MPa, 332.2 MPa

and 336.8 MPa, and the corresponding ·s were 322.9 MPa,

332.9 MPa and 337.8 MPa respectively, the maximum prediction error for the three strain amplitudes was 1.2 MPa. Although for the given strain range, ·c presented

relatively larger values compared with·satﬁrst then showed

relatively smaller values as the strain amplitude gradually increased, the predicted and actual stabilized cyclic stresses were approximately close to each other. Therefore, the universal feasibility of the prediction method was prelimi-narily veriﬁed. Meanwhile, the method could be appropriate for other structural materials with typical cyclic hardening behaviors, and from engineering standpoint, the testing work amount of cyclic stress-strain curve could be further reduced to a great extent.

4. Conclusions

A novel prediction method of low cyclic stress-strain curve for structural materials was investigated. The prediction method was based on a modiﬁed exponentialﬁtting equation, which was veriﬁed more appropriate to describe the low cyclic stress-strain curve than the known Hollomon equation. Based on the obtained results the following conclusions can be drawn.

(1) A miniaturized self-made device with separate modular tensile and fatigue actuators was developed to obtain the engineering and cyclic stress-strain curve curves. The tensile and fatigue actuators were respectively driven by servo motor and piezoelectric actuator. (2) A modiﬁed exponentialﬁtting equation and a prediction

method based on monotonic engineering stress-strain curve were proposed and discussed. Theoretically, the cyclic stress-strain curve could be deduced by merely three stabilized cyclic stresses at respective strain amplitude.

(3) A prediction method of cyclic stress-strain curve, which merely required the material’s two stabilized cyclic stresses at respective strain amplitudes and the engi-neering stress-strain curve, was proposed. For the extruded AZ31B magnesium alloy at the given strain amplitudes range from 0.0058 to 0.02, the ﬁtted and actual low cyclic stress-strain curves were approximate with correlation coefﬁcient of 0.9986. For 7075 aluminum alloy and H63 copper zinc alloy, the predicted and actual stabilized cyclic stresses were approximately close to each other. Therefore, the universal feasibility of the prediction method was preliminarily veriﬁed. Meanwhile, the method could be appropriate for other structural materials with typical cyclic hardening behaviors.

Acknowledgements

This research is funded by the National Natural Science

Fig. 5 Veriﬁcation of the prediction method by comparing with the actual low cyclic stress-strain curve.

**(a)**

**(b)**

1) G. E. Dieter:Mechanical Metallurgy, 3rd edition,119(McGraw-Hill, New York, 2009).

2) S. K. Paul, S. Majumdar and S. Kundu: Mater. Des.31(2012) 4386 4391.

3) G. S. Huang, J. H. Li, T. Z. Han, H. Zhang and F. S. Pan:Mater. Des.

58(2014) 439444.

12) S. Morita, S. Tanaka, M. Nakahara, N. Ohno, Y. Kawakami and T. Enjoji: J. Jpn. Met.59(2009) 548554.

13) Z. C. Ma, H. W. Zhao, H. B. Cheng and J. P. Li:Meas. Sci. Technol.25

(2014) 115011.